Adhesives technology 4
1-1 Introduction 4
A few words about adhesives 4
Huntsman industrial adhesives 5
Designing to bond 5
1-2 Assessment of bonding 6
Advantages of adhesive bonding 6
Adhesive types and main characteristics 10
1-3 Designing a bonded joint 12
Loading conditions 12
Determination of simple lap joints dimensions 20
Durability of a bonded joint 22
Bonding process essentials 24
A few words
This guide is designed to help engineers overcome the
reservations they may sometimes have about adhesives. It
includes a survey of modern adhesives and shows how joints
should be designed and pretreated in order to make the best
use of adhesive bonding. This guide has roots going back to
the days when adhesives capable of bonding metals were
first invented: our Araldite®
adhesive trade name is known
and recognised worldwide in both the industry and in the
The question about what is one trying to accomplish when
using an adhesive is not new. Man has used adhesives
or glues since the dawn of history. The ancient Egyptians
attached veneers to furniture with glue. These early glues
were all natural substances. Nowadays synthetic resins and
polymers are being used.
When components are bonded together, the adhesive first
thoroughly wets the surfaces to be bonded together filling
the gap in between and then starts to polymerize. When
hardening is complete, the bond can withstand the stresses
of use. High performance adhesives harden through chemical
reaction and have a strong affinity to joint surfaces. Adhesive
bonding is sometimes called chemical joining to differentiate it
from mechanical joining.
Just about every industrial item produced is
composed of components which have to be
assembled together. Mechanical fasteners such
as screws, rivets or spot welds are frequently
However, engineers now often choose to use
adhesive bonding. This assembly technique
is well proven and capable of replacing or
supplementing mechanical fastening methods
and can provide some advantages which
> Outstanding lap shear strength and peel
Reduced component and/or assembly costs
Improved product performance and durability
Greater design freedom
Less finishing operations
Adhesives have been used very successfully for years in
many very demanding industries, like aerospace, automotive,
wind energy, sport and leisure, railways, construction or
Our industrial adhesives form extremely strong and durable
bonds with plastics, metals, glass, rubber and many other
materials. Designers in just about every industry increasingly
find that bonding with Huntsman adhesives provides the
answer to production problems created by new materials,
new uses of existing materials, and new techniques and
Our industrial adhesives are easy to use, but to ensure
successful bonding the directions given in the instructions
supplied with the adhesive must be strictly followed.
1. Resin and hardener components must be measured in the
correct ratio as mentioned in our technical datasheets and
thoroughly mixed together.
2. Joint surfaces must be degreased and, when necessary,
3. Minimum curing temperature and curing time must be
observed (data given in the technical datasheets).
4. Jigs or other fixtures must be used to prevent the bond
surfaces from moving relative to one another during the
5. Though only light pressure is needed, it should be applied
as evenly as possible over the whole bond area. Excessive
pressure leaves the joint starved of adhesive.
Designing to bond
In order to get the best performance from an adhesive bond,
it is important to design the component for bonding rather
than simply taking a design made for mechanical fastening.
Methods of application of the adhesive and the assembly of
the components, must always be considered at the design
stage. Together, with the practical curing conditions, these
determine the choice of adhesive type to be used.
A quality bond can only be produced when quality is
considered at all stages of the design and production
The stress is uniformly distributed over the entire bond
area when a load is applied whereas the stress is highly
concentrated in a few areas when spot welding or
mechanical fasteners are used. Bonded assemblies will
therefore typically provide a longer service life under load.
Stiffer structures (Figure 1)
The continuity of a bonded assembly will produce stiffer
structures. Alternatively, if increased stiffness is not needed,
the weight of the structure can be decreased while
maintaining the required stiffness.
Adhesive bonding gives a smooth appearance to designs.
There are no protruding fasteners such as screws or rivets,
and no spot welds marks.
Jointing sensitive materials
Adhesive bonding does not require high temperatures. It is
highly suitable for joining together heat sensitive materials
prone to distortion or to a change in properties resulting from
the heat of brazing or welding processes.
Complex assemblies can often not be joined together by any
other fastening technique. Composite sandwich structures
being a typical example.
Adhesives can join different materials together – materials
that may differ in composition, moduli, coefficients of thermal
expansion, or thickness.
The continuous adhesive bond forms a seal. The joint is
consequently leak proof and less prone to corrosion.
1-2 Assessment of bonding
Reduced stress concentrations (Figure 2)
A bonded structure is inherently a safer structure because
the fewer and less severe concentrations of stresses are less
likely to induce fatigue cracks. Fatigue cracks will propagate
more slowly in a bonded structure than in a riveted structure
– or even in a machined profile because the bond lines will
typically stop crack formation.
The adhesive bond can provide an electrically insulating
barrier between the surfaces.
Some adhesives are specifically formulated to offer high
electrical conductivity (specially for electronic applications).
Adhesive bonds have good dampening properties which may
be useful for reducing sound or vibration.
Adhesive bonding can simplify assembly procedures by
replacing several mechanical fasteners with a single bond,
or by allowing several components to be joined in one
Adhesive bonding may be used in combination with spot
welding or mechanical fastening techniques in order to
improve the performance of the complete structure. All these
advantages may ultimately translate into improved economic
advantages: simplified design, easier assembly, lighter weight
(reduced energy utilisation), extended service life.
Fig.1 Stiffening effect - Bonding and
X = unstiffened area
The diagram shows how a joint may be designed to take
advantage of the stiffening effect of bonding. Adhesives form a
continuous bond between the joint surfaces. Rivets and spot
welds pin the surfaces together only at specific points. Bonded
structures are consequently much stiffer and loading may be
increased (by up to 30 - 100%) before buckling occurs.
Fig.2 Stress distribution
in loaded joints
The riveted joint at the top is highly stressed in the vicinity of the
rivets. Failure tends to initiate in these areas of peak stress. A
similar distribution of stress occurs with spot welds and bolts.
The bonded joint at the bottom is uniformly stressed. Likewise,
stress will be uniformly distributed in a welded joint, however
changes in the metal structure and strength will have taken
place in the vicinity of the weld.
1-2 Assessment of bonding
Adhesives are drawn from the class of materials known as
‘polymers’, ‘plastics’ or ‘synthetic resins’ and therefore have
their inherent limitations. They are not as strong as metals
however the difference is offset by the increased surface
contact area provided by the bonded joints. With increasing
temperature the bond strength decreases and the strain
properties of the adhesive move from elastic to plastic. This
transition is usually in the temperature range 70 – 220°C: the
transition temperature depends on the particular adhesive.
The resistance of bonded joints to the in-service environment
is dependent on the properties of the polymer from which the
adhesive is made. Possible exposure of the bonded structure
to oxidizing agents, solvents, etc., must be kept in mind
when selecting the adhesive type to use.
With most adhesives maximum bond strength is not
produced instantly as it is with mechanical fastening or with
welding. The bonded assembly must be supported while the
bond strength is developing.
The quality of the bond may be adversely affected if the
surfaces are not readily wetted by the adhesive during the
bonding process (see part 2 of this guide).
Ensuring consistently good results may necessitate the
setting up of unfamiliar process controls. A poorly executed
bonding is often impossible to correct.
In service repair
Bonded assemblies are usually not easily dismantled for
The main types of adhesives typically used in industry today
Anaerobic adhesives harden when in contact with metal
and air is excluded, e.g. when a screw is tightened in a
thread. Often referred to as ‘locking compounds’or ‘thread
sealants’, they are used to secure, seal and retain machined,
threaded, or similarly close-fitting parts. They are based on
synthetic resins known as acrylics. Due to the curing process,
anaerobic adhesives do not have gap-filling capability but
offer the advantage of relatively rapid curing.
A special type of acrylic, cyanoacrylate adhesives cure
through reaction with moisture held on the surfaces to be
bonded. They need close fitting joints. Usually they solidify in
seconds and are suited to small plastic parts and to rubber.
Cyanoacrylate adhesives have relatively little gap filling
capability but can be obtained in liquid and thixotropic (non-
Toughened acrylics / methacrylates
These adhesives based on a modified type of acrylic, are
fast curing and offer high strength and toughness. Supplied
as two parts (resin and catalyst), they are usually mixed
immediately before application. Some more specialised types
are also available where the components can be applied in
separate operations: the resin component to one surface to
be bonded, the catalyst to the other. They tolerate minimal
surface preparation and bond well to a wide range of
materials. The products are available in a wide range of cure
speeds and as liquids or pastes.
1-2 Assessment of bonding
Adhesive types and
Adhesives are classified either by the way they
are used or by their chemical type.
High performance adhesives harden via a
chemical reaction whereas lower performance
types typically harden via a simple physical
UV curable adhesives
Specially modified acrylic and epoxy adhesives, which can
be cured very rapidly by exposure to UV radiation. Acrylic
UV adhesives cure extremely rapidly on exposure to UV, but
require one substrate to be UV transparent. The UV initiated
epoxy adhesives can be irradiated before closing the bond
line, and cure in a few hours at ambient temperature or may
be cured at elevated temperatures.
Epoxy adhesives consist of an epoxy resin and a hardener.
With many resins and different hardeners to choose from,
they allow great versatility in formulation. They also form
extremely strong durable bonds with most materials. Epoxy
adhesives are available in one-component or two-component
form and can be supplied as flowable liquids, as highly
thixotropic products with gap filling capability of up to 25 mm,
as films or even in powder form.
Polyurethane adhesives are typically one-component
moisture curing or two-component systems. They provide
strong resilient joints, which are resistant to impacts. They are
useful for bonding FRP (fibre-reinforced plastics) and certain
thermoplastic materials and can be made with a range of
curing speeds and supplied as liquids or as pastes with gap
filling capability of up to 25 mm.
First adhesives for metals, modified phenolics now have
a long history of successful use for the production of high
strength metal to metal and metal to wood assemblies, and
for bonding metal to brake lining materials. Modified phenolic
adhesives require heat and high pressure for the curing
The above types cure through chemical reactions. The
following adhesive types are less performing, but still widely
used in industrial applications:
Related to sealing wax, which is one of the oldest forms of
adhesive, today’s industrial hot melts are based on modern
polymers. Hot melts are used for the fast assembly of
structures designed to be subjected to only light loads.
Plastisol adhesives are modified PVC dispersions which
require heat to harden. The resultant joints are often resilient
Based on solutions of latexes, rubber adhesives harden
through solvent or water evaporation. They are not suitable
for sustained loading.
Polyvinyl acetates (PVAs)
Vinyl acetate is the principal constituent of the PVA emulsion
adhesives. They are suitable for the bonding of porous
materials, such as paper or wood, and general packaging
Pressure sensitive adhesives
Typically used with tapes and labels, pressure sensitive
adhesives are designed to remain tacky and do not harden
but are often able to withstand adverse environments. They
are not suitable for sustained loading.
No one company supplies all these types of adhesives. Each
supplier specialises in particular types.
Huntsman Advanced Materials supplies many industries
with epoxy, polyurethane, modified phenolic, toughened
methacrylate and UV curable acrylic adhesives under the
trade names Araldite®
1-3 Designing a bonded joint
Bonded assemblies may be subjected to tensile,
compressive, shear or peel stresses, or a combination
thereof (Figure 3). Adhesives are more resilient under shear,
compression and tension stresses. They perform less
effectively under peel and cleavage loading. A bonded joint
needs to be designed so that the loading stresses will be
directed along the lines of the adhesive’s greatest strengths.
To indicate the typical performance properties to be expected
from a structural adhesive, the Huntsman Advanced Materials
technical data sheet for the particular adhesive will usually
report shear strengths and peel strengths obtained using
standard test methods.
For example, the standard test method for shear (ISO 4587)
uses a simple lap joint made from metal sheet, usually an
aluminum alloy, 25 mm wide with 12.5 mm overlap. The
mean breaking stress at room temperature will be in the
range 5 to 45 N/mm2
depending on the adhesive. At the top
end of this breaking stress range, assemblies made from
aluminum alloy sheet of up to 1.5 mm thickness will often
cause the substrate to yield or break. (The lap joint is only
one of several different types of bonded assemblies).
The breaking load of a lap joint is proportional to its width,
but not to its overlap length. Although the breaking load will
increase as overlap length is increased, the mean breaking
stress will be reduced.
A method of determining the best dimensions for a simple lap
joint is described in next chapter (Determination of simple lap
joints dimensions, p.20). The strength of a joint is a complex
function of the stress concentrations set up by the load. In
a simple lap joint made from thin metal sheet there are two
sorts of stress: shear and peel. Both the shear and peel
stresses vary along the length of the joint, with concentrations
at the ends. Alternative joint designs are shown thereafter
where these stresses are more evenly distributed (Figure 4).
The efficiency gained results in joints of greater strength.
It is critical that an assembly which will
ultimately be bonded is designed with bonding
in mind, rather than simply bonding a design
intended for welding or mechanical fastening.
When designing bonded joints the following
aspects must be considered:
Adhesive performance properties
Stress in the joint
Fig.3 Loading conditions
A bonded joint can be loaded in five basic ways (as shown in the diagrams above). Cleavage and peel loading are the most severe
as they concentrate the applied force into a single line of high stress. In practice, a bonded structure has to sustain a combination of
forces. For optimum strength, the bonded assembly should be designed in such a way as to avoid cleavage and peel stresses.
1-3 Designing a bonded joint
Fig.4 Basic bonded joints between strip / sheet metals
A peel joint can be designed such that the forces acting on it
become compression forces, making a much stronger joint.
Weak cleavage joints can be strengthened through design, in this
instance by adding a U-section to the previously bent sheet.
The basic types of bonded joints are shown in the diagrams
above. In practice, a combination of two or more basic types
may be used – and the relative dimensions (and areas of
bonded surface) of the joints may vary from those shown in
the diagrams. Tapering of the ends of lap joints or scarf joints
serves to distribute the stress more uniformly and reduce stress
By adding a reinforcing plate to this butt joint, the forces run along a
much stronger shear joint.
A similar effect is produced by sleeving this cylindrical butt joint.
Simple lap joint - good.
Scarf joint - excellent.
Double strap joint / double lap joint - very good.
Tapered lap joint - very good.
Stepped lap joint - very good.
Tapered double strap joint - excellent.
1-3 Designing a bonded joint
Fig.5 Practical bonded joints between sheet materials
Fig.6 Bonding of multi-layer structures
Multi-layer structures may be built up by adhesive bonding
and may also be bonded to other parts. In (A) a multi-layer
fibre-reinforced plastics laminate is joined to its neighbour by a
multi-stepped lap joint. In (B) an edge member is bonded into
a sandwich panel. On loading, the stresses will be transferred
into the panel. The honeycomb core is itself assembled and
bonded to the facing sheets with adhesives.
1-3 Designing a bonded joint
Fig.7 Joints using profiles
Sheets or plates that cannot be bent and folded may be
bonded together by means of purpose-made profiles. Tapering
removes the high stress concentrations caused by abrupt
change in section.
Fig.8 Stiffening of large thin sheets
Large sheets of thin gauge material (metal or plastics) may be
stabilised by bonding stiffeners made of the same material in
similar gauge. The diagram shows a ‘top hat’ stiffener. Towards
the edge of the sheet, the stiffener may be cut away (as shown)
in order to reduce stress concentrations. The effect is similar to
that of the scarf joint (Figure 4).
Fig.9 Bonded frameworks
A. Plug design
C. Boss design
B. Angle design
Framework structures of square or round tubes, or simple
profiles, may utilise plugs (A), angles (B), or bosses (C) at the
joints. Use of these additional pieces greatly increases the area
of bond surface at the joint.
1-3 Designing a bonded joint
The shear strength of simple lap joint (Figure 10) depends
on the nature of the metal, the adhesive, the thickness of the
metal and the area of overlap.
Given the loading required and the metal and adhesive to be
used, it is possible to predict:
1. Optimum overlap on metals of given thickness.
2. Optimum metal thickness for given overlap.
This overlap and thickness may be rapidly determined from a
diagram based on results from one test program.
The test - to determine mean shear strengths of joints
of various overlaps (l) and metal thickness (t) - must be
sufficient to plot a curve of shear strength against t/l. A curve
established in this way is shown thereafter (Figure 11).
Any particular point on an established curve represents
(for lap joints made with metal and adhesive to the same
specifications as used in the test program) the state of stress
in a particular joint and shows the relationship between the
dimensions of the joint (horizontal axis), the mean shear
stress in the adhesive (vertical axis) and the mean tensile
stress in the metal (slope of a straight line from the origin to
Optimum overlap (l) is determined by using the diagram
together with the formula: τ = σ . t/l
This formula is derived from the known design requirements:
P = load per unit width of joint
t = sheet thickness (t= thickness of thinner sheet in joints
made of sheets of different thickness)
σ = mean tensile stress in the metal = P/t and by definition:
τ= mean shear stress in the joint = P/l
Substituting for P gives: τ = σ . t/l (Figure 12).
simple lap joints
Optimum overlap (l) is determined as follows:
1. Calculate σ from P and t.
2. Starting from 0, mark on the diagram the straight line
whose slope (τ / t/l) is given by σ.
3. Where the straight line cuts the curve, read off the value for
4. Having determined σ and τ, and knowing t, substitute
these values in: τ = σ . t/l and calculate optimum overlap l.
Deviation from the optimum overlap reduces the efficiency of
the joint. A too small overlap causes the joint to fail below the
required loading, whereas a too large overlap may mean an
unnecessarily large joint.
Optimum sheet thickness (t) is determined as follows:
1. Calculate τ from P and l.
2. Where the value of t cuts the curve, read off the value for
3. Having determined t/l and knowing l, calculate optimum
Fig.10 Simple lap shear joint
Fig.11 Correlation diagram
between shear strength and t/l of simple lap joints
The diagram relates the dimensions of the joint, the shear
stress in the adhesive and the tensile stress in the metal. The
curve shown was established from a test program carried out
on simple lap joints of BS 1470-HS30 aluminum alloy bonded
with hot-cured Araldite®
Fig.12 Conventional designs for
stresses in a lap joint
0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 1.0
Mean failure stress (N / mm2
t/l ratio of lap joint
l = overlap I t = metal thickness
1-3 Designing a bonded joint
This necessitates control of pretreatment of the surfaces (part
2 of this guide). A poor surface condition usually results in a
relatively low initial strength and a reduced durability. A thick
bond line gives lower initial strength (Figure 13). With most
types of adhesive, the application of heat to complete the
curing process improves both initial strength and durability.
The user will have to assess the level of control of these
factors necessary to produce a bonded joint satisfactory
for the expected service conditions. For many applications
a good and sufficient durability is obtained with easily
achievable levels of surface control (or pretreatment), bond
line thickness and curing schedule.
Shear strength decreases if the layer of adhesive is thick.
The effect of increasing bond line thickness in simple lap
joints made with hot cured epoxy adhesives is shown in the
diagram (Figure 13).
The optimum bond line thickness is in the range 0.1 to 0.3
mm. In very thin bond lines there is risk of incomplete filling
of the joint due to contact between high points on the joint
The bonded joints may need to resist sustained loads, which
are either static or vibrational. Joint designs in which peel
stresses are at a minimum give the best durability. The fatigue
testing (by standard methods) of simple lap shear joints made
with epoxy adhesives will often give failure values of ca 30%
of the short term measured breaking load (Figure 14).
Durability of a
The long-term performance of a bonded joint
depends on the properties both of the adhesive
and of the materials being joined. The adhesive
will be affected by high temperatures, by
powerful solvents or by water.
The durability of the joint will also depend on the
effects of these agents on the materials being
joined. Above all, it will depend on the condition
of the joint surfaces when the bond was made.
The best joints are made when the surfaces are
absolutely clean and have good affinity to the
Fig.13 Bond line thickness
vs. shear strength
Adhesive strength at the interface is by its nature greater
than the cohesive strength within the adhesive. The diagram
shows that in this adhesive the drop in strength occurs in the
range 0.4 to 1.0 mm. In thicknesses greater than 1.0 mm
shear strength is approximately constant. The exact shape
of the curve depends on the characteristics of the adhesive.
Toughened adhesives will maintain higher values in thicker bond
lines while more rigid adhesives will decline more quickly.
Fig.14 Fatigue strength (tensile)
of lap joints
Fatigue strength of simple lap joints made with a cold cured
epoxy adhesive and tested to DIN 53 285. In this test
programme, the failure stress of control joints under static
loading was 10 MPa. The diagram shows that under fatigue
loading the joints required to sustain 106
test cycles should not
be stressed higher than 3.6 MPa per cycle.
0 0.4 0.8 1.2
Failure stress (MPa)
Bond-line thickness (mm)
% of static failure stress
Cycles to failure
Maximum stress level (MPa)
With a two-component adhesive this means that resin and
hardener must be thoroughly mixed in the correct ratio.
An appropriate amount of mixed adhesive needs to be
placed and spread onto the bond area. Both steps can
be performed with automatic equipment. The simplest
equipment dispenses adhesive from pre-filled cartridges
(Figure 15 and 16). An example of a typical mix-metering
equipment, which meters, mixes and dispenses two-
component adhesives is shown (Figure 17).
Where highly viscous or thixotropic components are used,
the metering units may be fed by special drum pumps.
Similarly for single component epoxy adhesives there are
hand or air operated application equipment. Well designed
and maintained application equipment will help ensure
a reproducible and dependable quality bond. Suitable
equipment is advantageous in setting up a Quality Assurance
Scheme for a bonding process.
The continuous bonding process also requires a uniform and
consistent surface preparation. All foreign contaminants must
be removed from the surfaces. A particular surface treatment
may be needed in order to improve the affinity for the
adhesive. Surface preparation can be a multi-step process
and typically includes mechanical abrasion and - to achieve
optimum results - chemical etching (Part 2 of this guide).
In some instances known surface contaminants such as
protective oils, may be absorbed by the adhesive in the
bonding process – this ability is a characteristic of specially
formulated oil-tolerant adhesives. In these cases the present
contaminants define the surface condition.
The hardening or curing of reactive adhesives requires time.
The time is shortened if heat can be applied. Furthermore,
although strong bonds can be achieved after 2 to 24 hours
at room temperature curing with many two-part adhesives,
exposing the adhesive bond to higher curing temperatures
– even a few degrees above room temperature – will usually
increase the bond strength.
1-3 Designing a bonded joint
To make a successful bond, the adhesive must
wet the surfaces to be assembled, fill the gap
between the two surfaces, and then fully cure.
With some specific single component epoxy adhesives,
curing temperatures as high as 180°C may be required in
order to obtain the optimum properties. Elevated temperature
curing may be carried out using:
Hot air ovens
This is a practical method only when a large number of
assemblies are in the oven at the same time or for continuous
production lines. Heat transfer is relatively slow and affected
by the assembly type and thickness. Infrared ovens can also
Steam or oil-heated platens can be used in flat bed presses
with a rapid and controllable temperature rise. This method
is ideal for production of large flat panels, e.g. for insulated
container side panels.
Magnetic field causes current to flow in a conductive
substrate. The resistance to the current generates heat and
cures the adhesive. This technique has been used where very
fast heat up and cure is required.
Fig.15 Manual applicators
dedicated to different cartridges sizes
Fig.16 Different types and sizes
of easy to use packaging for Huntsman industrial adhesives
Fig.17 Mix-metering equipment
for two-component adhesives (courtesy of DOPAG AG)